LMucko/crystallography-open-database huggingface dataset:
The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene Sample: P = 0 GPa, in air
Nestola, F.; Ballaran, T. B.; Balic-Zunic T; Secco, L.; Dal Negro, A.; American Mineralogist 93 (2008) 644–652; doi:10.2138/am.2008.2693

data_9010424
_publ_section_title
;
 The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene
 Sample: P = 0 GPa, in air
;
_journal_name_full               'American Mineralogist'
_journal_page_first              644
_journal_page_last               652
_journal_paper_doi               10.2138/am.2008.2693
_journal_volume                  93
_journal_year                    2008
_chemical_formula_sum
'Al0.236 Ca0.01 Fe0.967 Mg0.923 Mn0.016 O6 Si1.848'
_chemical_name_mineral           Orthopyroxene
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   18.2889
_cell_length_b                   8.8662
_cell_length_c                   5.2175
_cell_formula_units_Z            8
_cell_volume                     846.034
_database_code_amcsd             0004556
_diffrn_ambient_pressure         0
_exptl_crystal_density_diffrn    3.643
_cod_original_formula_sum
'Fe.967 Mg.923 Ca.01 Mn.016 Al.236 Si1.848 O6'
_cod_database_code               9010424
The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene Sample: P = 0 GPa, in air, same # of reflections as DAC crystal
Nestola, F.; Ballaran, T. B.; Balic-Zunic T; Secco, L.; Dal Negro, A.; American Mineralogist 93 (2008) 644–652; doi:10.2138/am.2008.2693

data_9010425
_publ_section_title
;
 The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene
 Sample: P = 0 GPa, in air, same # of reflections as DAC crystal
;
_journal_name_full               'American Mineralogist'
_journal_page_first              644
_journal_page_last               652
_journal_paper_doi               10.2138/am.2008.2693
_journal_volume                  93
_journal_year                    2008
_chemical_formula_sum
'Al0.236 Ca0.01 Fe0.967 Mg0.923 Mn0.016 O6 Si1.848'
_chemical_name_mineral           Orthopyroxene
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   18.2889
_cell_length_b                   8.8662
_cell_length_c                   5.2175
_cell_formula_units_Z            8
_cell_volume                     846.034
_database_code_amcsd             0004557
_diffrn_ambient_pressure         0
_exptl_crystal_density_diffrn    3.643
_cod_original_formula_sum
'Fe.967 Mg.923 Ca.01 Mn.016 Al.236 Si1.848 O6'
_cod_database_code               9010425
The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene Sample: P = 0.163 GPa
Nestola, F.; Ballaran, T. B.; Balic-Zunic T; Secco, L.; Dal Negro, A.; American Mineralogist 93 (2008) 644–652; doi:10.2138/am.2008.2693

data_9010426
_publ_section_title
;
 The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene
 Sample: P = 0.163 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              644
_journal_page_last               652
_journal_paper_doi               10.2138/am.2008.2693
_journal_volume                  93
_journal_year                    2008
_chemical_formula_sum
'Al0.236 Ca0.01 Fe0.967 Mg0.923 Mn0.016 O6 Si1.848'
_chemical_name_mineral           Orthopyroxene
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   18.2804
_cell_length_b                   8.8601
_cell_length_c                   5.2161
_cell_formula_units_Z            8
_cell_volume                     844.832
_database_code_amcsd             0004558
_diffrn_ambient_pressure         1.63e+05
_exptl_crystal_density_diffrn    3.648
_cod_original_formula_sum
'Fe.967 Mg.923 Ca.01 Mn.016 Al.236 Si1.848 O6'
_cod_database_code               9010426
The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene Sample: P = 1.715 GPa
Nestola, F.; Ballaran, T. B.; Balic-Zunic T; Secco, L.; Dal Negro, A.; American Mineralogist 93 (2008) 644–652; doi:10.2138/am.2008.2693

data_9010427
_publ_section_title
;
 The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene
 Sample: P = 1.715 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              644
_journal_page_last               652
_journal_paper_doi               10.2138/am.2008.2693
_journal_volume                  93
_journal_year                    2008
_chemical_formula_sum
'Al0.236 Ca0.01 Fe0.967 Mg0.923 Mn0.016 O6 Si1.848'
_chemical_name_mineral           Orthopyroxene
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   18.2192
_cell_length_b                   8.8111
_cell_length_c                   5.1965
_cell_formula_units_Z            8
_cell_volume                     834.200
_database_code_amcsd             0004559
_diffrn_ambient_pressure         1.715e+06
_exptl_crystal_density_diffrn    3.694
_cod_original_formula_sum
'Fe.967 Mg.923 Ca.01 Mn.016 Al.236 Si1.848 O6'
_cod_database_code               9010427
The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene Sample: P = 3.947 GPa
Nestola, F.; Ballaran, T. B.; Balic-Zunic T; Secco, L.; Dal Negro, A.; American Mineralogist 93 (2008) 644–652; doi:10.2138/am.2008.2693

data_9010428
_publ_section_title
;
 The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene
 Sample: P = 3.947 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              644
_journal_page_last               652
_journal_paper_doi               10.2138/am.2008.2693
_journal_volume                  93
_journal_year                    2008
_chemical_formula_sum
'Al0.236 Ca0.01 Fe0.967 Mg0.923 Mn0.016 O6 Si1.848'
_chemical_name_mineral           Orthopyroxene
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   18.1427
_cell_length_b                   8.7460
_cell_length_c                   5.1716
_cell_formula_units_Z            8
_cell_volume                     820.609
_database_code_amcsd             0004560
_diffrn_ambient_pressure         3.947e+06
_exptl_crystal_density_diffrn    3.755
_cod_original_formula_sum
'Fe.967 Mg.923 Ca.01 Mn.016 Al.236 Si1.848 O6'
_cod_database_code               9010428
The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene Sample: P = 8.033 GPa
Nestola, F.; Ballaran, T. B.; Balic-Zunic T; Secco, L.; Dal Negro, A.; American Mineralogist 93 (2008) 644–652; doi:10.2138/am.2008.2693

data_9010429
_publ_section_title
;
 The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene
 Sample: P = 8.033 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              644
_journal_page_last               652
_journal_paper_doi               10.2138/am.2008.2693
_journal_volume                  93
_journal_year                    2008
_chemical_formula_sum
'Al0.236 Ca0.01 Fe0.967 Mg0.923 Mn0.016 O6 Si1.848'
_chemical_name_mineral           Orthopyroxene
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   18.0221
_cell_length_b                   8.6456
_cell_length_c                   5.1327
_cell_formula_units_Z            8
_cell_volume                     799.736
_database_code_amcsd             0004561
_diffrn_ambient_pressure         8.033e+06
_exptl_crystal_density_diffrn    3.853
_cod_original_formula_sum
'Fe.967 Mg.923 Ca.01 Mn.016 Al.236 Si1.848 O6'
_cod_database_code               9010429
The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene Sample: P = 9.562 GPa
Nestola, F.; Ballaran, T. B.; Balic-Zunic T; Secco, L.; Dal Negro, A.; American Mineralogist 93 (2008) 644–652; doi:10.2138/am.2008.2693

data_9010430
_publ_section_title
;
 The high-pressure behavior of an Al- and Fe-rich natural orthopyroxene
 Sample: P = 9.562 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              644
_journal_page_last               652
_journal_paper_doi               10.2138/am.2008.2693
_journal_volume                  93
_journal_year                    2008
_chemical_formula_sum
'Al0.236 Ca0.01 Fe0.967 Mg0.923 Mn0.016 O6 Si1.848'
_chemical_name_mineral           Orthopyroxene
_space_group_IT_number           61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   17.9770
_cell_length_b                   8.6100
_cell_length_c                   5.1227
_cell_formula_units_Z            8
_cell_volume                     792.902
_database_code_amcsd             0004562
_diffrn_ambient_pressure         9.562e+06
_exptl_crystal_density_diffrn    3.887
_cod_original_formula_sum
'Fe.967 Mg.923 Ca.01 Mn.016 Al.236 Si1.848 O6'
_cod_database_code               9010430
Synchotron powder X-ray diffraction study of the structure and dehydration behavior of palygorskite Sample: T = 100 K
Post, J. E.; Heaney, P. J.; American Mineralogist 93 (2008) 667–675; doi:10.2138/am.2008.2590

data_9010431
_publ_section_title
;
 Synchotron powder X-ray diffraction study of the structure and dehydration
 behavior of palygorskite
 Sample: T = 100 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              667
_journal_page_last               675
_journal_paper_doi               10.2138/am.2008.2590
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        'Yulu River, Korea'
_chemical_formula_sum            'Al1.1 H9 Mg O14.92 Si3.9'
_chemical_name_mineral           Palygorskite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.77
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.179
_cell_length_b                   17.852
_cell_length_c                   5.2316
_cell_volume                     1172.122
_database_code_amcsd             0004563
_diffrn_ambient_temperature      100
_exptl_crystal_density_diffrn    2.331
_cod_original_formula_sum        'Al1.1 Mg Si3.9 O14.92 H9'
_cod_database_code               9010431
Synchotron powder X-ray diffraction study of the structure and dehydration behavior of palygorskite Sample: T = 300 K
Post, J. E.; Heaney, P. J.; American Mineralogist 93 (2008) 667–675; doi:10.2138/am.2008.2590

data_9010432
_publ_section_title
;
 Synchotron powder X-ray diffraction study of the structure and dehydration
 behavior of palygorskite
 Sample: T = 300 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              667
_journal_page_last               675
_journal_paper_doi               10.2138/am.2008.2590
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        'Yulu River, Korea'
_chemical_formula_sum            'Al2.2 H22 Mg2.14 O30 Si7.8'
_chemical_name_mineral           Palygorskite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.560
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   13.2858
_cell_length_b                   17.8476
_cell_length_c                   5.2419
_cell_volume                     1185.038
_database_code_amcsd             0004564
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    2.333
_cod_original_formula_sum        'Al2.2 Mg2.14 Si7.8 O30 H22'
_cod_database_code               9010432
Synchotron powder X-ray diffraction study of the structure and dehydration behavior of palygorskite Sample: T = 1160 K
Post, J. E.; Heaney, P. J.; American Mineralogist 93 (2008) 667–675; doi:10.2138/am.2008.2590

data_9010433
_publ_section_title
;
 Synchotron powder X-ray diffraction study of the structure and dehydration
 behavior of palygorskite
 Sample: T = 1160 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              667
_journal_page_last               675
_journal_paper_doi               10.2138/am.2008.2590
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        'Lemesurier Island, Alaska'
_chemical_formula_sum            'Al Mg O10.4 Si4'
_chemical_name_mineral           Palygorskite
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 96.17
_cell_angle_gamma                90
_cell_length_a                   10.755
_cell_length_b                   15.353
_cell_length_c                   5.281
_cell_formula_units_Z            4
_cell_volume                     866.956
_database_code_amcsd             0004565
_diffrn_ambient_temperature      1160
_exptl_crystal_density_diffrn    2.528
_cod_original_formula_sum        'Al Mg Si4 O10.4'
_cod_database_code               9010433
Eskolaite associated with diamond from the Udachnaya kimberlite pipe, Yakutia, Russia Locality: natural diamond, Udachnaya pipe, Yukutia, Russia
Logvinova, A. M.; Wirth, R.; Sobolev, N. V.; Seryotkin, Y. V.; Yefimova, E. S.; Floss, C.; Taylor, L. A.; American Mineralogist 93 (2008) 685–690; doi:10.2138/am.2008.2670

data_9010434
_publ_section_title
;Eskolaite associated with diamond from the Udachnaya kimberlite pipe,
 Yakutia, Russia Locality: natural diamond, Udachnaya pipe, Yukutia, Russia
;
_journal_name_full               'American Mineralogist'
_journal_page_first              685
_journal_page_last               690
_journal_paper_doi               10.2138/am.2008.2670
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source
'natural diamond, Udachnaya pipe, Yukutia, Russia'
_chemical_formula_sum            'Al0.058 Cr1.702 Fe0.122 Mg0.042 O3 Ti0.076'
_chemical_name_mineral           Eskolaite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.9696
_cell_length_b                   4.9696
_cell_length_c                   13.597
_cell_formula_units_Z            6
_cell_volume                     290.815
_database_code_amcsd             0004566
_exptl_crystal_density_diffrn    5.123
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        '(Cr1.702 Fe.122 Ti.076 Al.058 Mg.042) O3'
_cod_database_code               9010434
Lakebogaite, CaNaFe3+2H(UO2)2(PO4)4(OH)2(H2O)8, a new uranyl phosphate with a unique crystal structure from Victoria, Australia Locality: Upper Devonian granite, near Lake Boga, northern Victoria, Australia
Mills, S. J.; Birch, W. D.; Kolitsch, U.; Mumme, W. G.; Grey, I. E.; American Mineralogist 93 (2008) 691–697; doi:10.2138/am.2008.2706

data_9010435
_publ_section_title
;Lakebogaite, CaNaFe3+2H(UO2)2(PO4)4(OH)2(H2O)8, a new uranyl phosphate with a
 unique crystal structure from Victoria, Australia Locality: Upper Devonian
 granite, near Lake Boga, northern Victoria, Australia
;
_journal_name_full               'American Mineralogist'
_journal_page_first              691
_journal_page_last               697
_journal_paper_doi               10.2138/am.2008.2706
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source
'Upper Devonian granite, near Lake Boga, northern Victoria, Australia'
_chemical_formula_sum
'Al0.09 Ca0.87 Fe1.91 H15.72 Na1.13 O29 P4 U1.888'
_chemical_name_mineral           Lakebogaite
_space_group_IT_number           9
_symmetry_space_group_name_Hall  'C -2yc'
_symmetry_space_group_name_H-M   'C 1 c 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.692
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   19.6441
_cell_length_b                   7.0958
_cell_length_c                   18.7029
_cell_volume                     2349.273
_database_code_amcsd             0004567
_exptl_crystal_density_diffrn    3.458
_cod_original_formula_sum
'U1.888 Fe1.91 Al.09 P4 Ca.87 Na1.13 O29 H15.72'
_cod_database_code               9010435
Crystal structure and Raman spectrum of hydroxyl-bastnasite-(Ce), CeCO3(OH) Note: changed Ce3(z) to .2579 according to authors Locality: Trimouns, Luzenac, France
Yang, H.; Dembowski, R. F.; Conrad, P. G.; Downs, R. T.; American Mineralogist 93 (2008) 698–701; doi:10.2138/am.2008.2827

data_9010436
_publ_section_title
;
 Crystal structure and Raman spectrum of hydroxyl-bastnasite-(Ce), CeCO3(OH)
 Note: changed Ce3(z) to .2579 according to authors
 Locality: Trimouns, Luzenac, France
;
_journal_name_full               'American Mineralogist'
_journal_page_first              698
_journal_page_last               701
_journal_paper_doi               10.2138/am.2008.2827
_journal_volume                  93
_journal_year                    2008
_chemical_formula_sum
'C H0.65 Ce0.5 F0.35 La0.23 Nd0.24 O3.65 Y0.03'
_chemical_name_mineral           Hydroxyl-bastnasite-(Ce)
_space_group_IT_number           174
_symmetry_space_group_name_Hall  'P -6'
_symmetry_space_group_name_H-M   'P -6'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            18
_cell_length_a                   12.4112
_cell_length_b                   12.4112
_cell_length_c                   9.8511
_cell_volume                     1314.144
_exptl_crystal_density_diffrn    4.936
_cod_original_formula_sum        '(Ce.5 Nd.24 La.23 Y.03) C O3.65 (F.35 H.65)'
_cod_database_code               9010436
_database_code_amcsd             0004568
Crystal structure and Raman spectrum of hydroxyl-bastnasite-(Ce), CeCO3(OH) Note: changed Ce3(z) to .2579 according to authors Locality: Trimouns, Luzenac, France
Yang, H.; Dembowski, R. F.; Conrad, P. G.; Downs, R. T.; American Mineralogist 93 (2008) 698–701; doi:10.2138/am.2008.2827

data_9010437
_publ_section_title
;
 Crystal structure and Raman spectrum of hydroxyl-bastnasite-(Ce), CeCO3(OH)
 Note: changed Ce3(z) to .2579 according to authors
 Locality: Trimouns, Luzenac, France
;
_journal_name_full               'American Mineralogist'
_journal_page_first              698
_journal_page_last               701
_journal_paper_doi               10.2138/am.2008.2827
_journal_volume                  93
_journal_year                    2008
_chemical_formula_sum
'C H0.65 Ce0.5 F0.35 La0.23 Nd0.24 O3.65 Y0.03'
_chemical_name_mineral           Hydroxylbastnasite-(Ce)
_space_group_IT_number           174
_symmetry_space_group_name_Hall  'P -6'
_symmetry_space_group_name_H-M   'P -6'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            18
_cell_length_a                   12.4112
_cell_length_b                   12.4112
_cell_length_c                   9.8511
_cell_volume                     1314.144
_exptl_crystal_density_diffrn    4.936
_cod_duplicate_entry             9010436
_cod_original_formula_sum        '(Ce.5 Nd.24 La.23 Y.03) C O3.65 (F.35 H.65)'
_cod_database_code               9010437
The crystal structure of vurroite, Pb20Sn2(Bi,As)22S54Cl6: OD-character, polytypism, twinning, and modular description
Pinto, D.; Bonaccorsi, E.; Balic-Zunic T; Makovicky, E.; American Mineralogist 93 (2008) 713–727; doi:10.2138/am.2008.2639

data_9010438
_publ_section_title
;
 The crystal structure of vurroite, Pb20Sn2(Bi,As)22S54Cl6: OD-character,
 polytypism, twinning, and modular description
;
_journal_name_full               'American Mineralogist'
_journal_page_first              713
_journal_page_last               727
_journal_paper_doi               10.2138/am.2008.2639
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        'Vulcano, Aeolian Islands, Italy'
_chemical_formula_sum            'As4.71 Bi6.97 Cl3 Pb9.6 S27 Sn0.72'
_chemical_name_mineral           Vurroite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.83
_cell_angle_gamma                90
_cell_length_a                   8.371
_cell_length_b                   45.502
_cell_length_c                   27.273
_cell_formula_units_Z            8
_cell_volume                     10265.091
_database_code_amcsd             0004570
_exptl_crystal_density_diffrn    6.285
_cod_original_cell_volume        10265.092
_cod_original_formula_sum        'Pb9.6 Bi6.97 As4.71 Sn.72 S27 Cl3'
_cod_database_code               9010438
Crystal chemistry of the natrojarosite-jarosite and natrojarosite-hydronium jarosite solid-solution: A synthetic study with full Fe site occupancy Sample: K
Basciano, L. C.; Peterson, R. C.; American Mineralogist 93 (2008) 853–862; doi:10.2138/am.2008.2731

data_9010439
_publ_section_title
;
 Crystal chemistry of the natrojarosite-jarosite and natrojarosite-hydronium
 jarosite solid-solution: A synthetic study with full Fe site occupancy
 Sample: K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              853
_journal_page_last               862
_journal_paper_doi               10.2138/am.2008.2731
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe3 H6 K0.76 Na0.24 O14 S2'
_chemical_name_mineral           Jarosite
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   7.3045
_cell_length_b                   7.3045
_cell_length_c                   17.0875
_cell_formula_units_Z            3
_cell_volume                     789.569
_database_code_amcsd             0004571
_exptl_crystal_density_diffrn    3.135
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_original_formula_sum        '(K.76 Na.24) Fe3 S2 O14 H6'
_cod_database_code               9010439